Ilia A Pankin

Houeida Issa Hamoud

Kirill A Lomachenko
email: lomachenko@esrf.fr

Søren Birk Rasmussen

Andrea Martini

Philippe Bazin

Valentin Valtchev

Marco Daturi
email: marco.daturi@ensicaen.fr

Carlo Lamberti

Silvia Bordiga

Cu-and Fe-speciation in composite zeolite catalyst for selective catalytic reduction of NO x : insights from operando XAS

Cu-SAPO-34 (Cu-CZC) and Fe-Mordenite (Fe-MOR) and their mechanical mixture (50:50) have been exhaustively investigated by means of operando X-ray absorption spectroscopy under NH3-SCR conditions. Fe K-edge XANES and EXAFS analysis revealed similar Fe-speciation in both pure Fe-MOR catalyst and the mechanical mixture after high-temperature pretreatment and under reaction conditions. In contrast, analysis of the Cu K-edge dataset unveiled essentially different trends in temperature-driven Cu-speciation in the pure Cu-CZC and mechanical mixture under standard NH3-SCR conditions. This difference is more evident in the low-temperature range. The presence of Fe-MOR counterpart in the mixed catalyst can result in the increase of NH3 an NO concentration in proximity of Cu-sites, which facilitates temperature-driven migration of NH3-solvated mobile di-amino complexes from Cu-CZC to the MOR framework. This decreases the density of mobile Cu I complexes in the entire system and results in the higher reducibility of Cu in the mixed catalyst. The obtained results help in understanding the precise speciation of the active sites in such composite catalysts and thus provides future guidance to design of such systems.

Introduction

NH 3 -assisted Selective Catalytic Reduction (NH 3 -SCR) catalyzed by metal-exchanged zeolites is a promising way to remove hazardous NO x from diesel engine exhaust gases 1-5 . The development of after-treatment catalysts able to abate NO x emissions, meeting the increasingly demanding air-quality EU standards, is an ongoing challenge, which nowadays attracts an enormous research interest from both academic and industrial laboratories, notably addressing the efficient zeolite-based SCR process [START_REF] Zhang | [END_REF] .

The reason to investigate the bimetallic catalysts is provided by the fact that Fe-exchanged zeolites were found to be highly active at high temperatures (T > 350 o C), while Cuzeolites demonstrate superior activity at low temperature SCR (T < 300 o C) [7][8][9][10][11][12] . In this regard, different complex system containing simultaneously copper and iron zeolites, such as dual-layer catalysts and Cu-Fe co-exchanged zeolites 8, 12-18 were thoroughly investigated in order to efficiently cover a broad temperature range. Moreover, additional interest to this kind of system is given by the fact that in few recent works the synergetic effect between Cu and Fe sites was proposed for different catalytic reactions. Hammond et al. 19, 20 reported an increase of the methanol selectivity for direct methane to methanol conversion over Fe-ZSM-5 catalysts caused by the presence of Cu II cations in the catalyst. The Fe and/or Cucontaining BEA zeolites prepared by two-step post-synthesis method and conventional wet impregnation have been studied for NH 3 -SCR applications 21 . It was shown that the co-presence of copper in the zeolite structure decreased the reducibility of iron and had significant influence on the low temperature NO conversion. The Cu-Fe/ZSM-5 catalyst, prepared by subsequent ion-exchange, showed higher NO x conversion compared with Fe/ZSM-5 or Cu/ZSM-5 due to the facile reduction of metal species 9 . The (Cu + Fe)-beta catalyst, prepared by solid-state ion-exchange method, showed higher NH 3 -SCR activity over a broader temperature range, and especially at low temperature as compared to the Fe-beta and Cu-beta counterparts 13 . Gao et al. 12 exhaustively investigated catalytic activity and selectivity under NH 3 -SCR conditions of the physical mixture of hydrothermally aged Cu-SSZ-13 and Fe-SSZ-13, revealing that such catalyst provide stable SCR performance in wide temperature range and essentially decrease N 2 O formation at high temperature. Metkar et al. This journal is © The Royal Society of Chemistry 20xx

Please do not adjust margins Please do not adjust margins of a thicker Cu-CHA layer at bottom gave maximum NO x reduction activities for the fast SCR reactions. While great research efforts have been done on the investigation of Mesites speciation in the monometallic exchanged zeolites under NH 3 -SCR conditions, complete understanding of both structural and electronic properties of the metallic active Cuand Fe-sites simultaneously present in the catalyst under SCR conditions is still an ongoing challenge. Furthermore, the synthesis of bimetallic zeolitic catalysts is a complex process which may involve few post-synthesis steps such as liquid and solid-state ion exchange or wet impregnation 9, 13, 21 . Therefore, we have recently proposed, as an alternative, the mechanical mixture of Cu and Fe-exchanged zeolites, which has shown superior catalytic performances respect to the average of the monometallic counterpart 22 . However, some questions remained open concerning the state of copper and iron inside the porous materials, as well as the synergy between the two cations (placed at a relatively long distance in the physical mixture, indeed) and the possible modification of the catalyst composition under stream. This requires a deeper insight into the chemical and physical properties of the materials during the catalytic action, which is the focus of the present study.

Recently the speciation of Cu-sites during high temperature pre-treatment and under NH 3 -SCR conditions has been studied using a combined in situ UV-vis, FTIR and XAS spectroscopies 23-26 , as well as by combining Cu K-edge XANES and XRPD Rietveld maximum entropy refinement 27 . Lomachenko et al. 28 , based on combined experimental XAS and valence-to-core XES investigations of Cu-SSZ-13 (Cu:Al = 0.48; Si:Al = 15), revealed the co-presence of Cu I /Cu II species with the predominance of mobile NH 3 -solvated complexes for low-temperature SCR (< ⁓200 о С), while higher Cu II fraction can be obtained at higher temperatures (> 350 °C). Tyrsted et al.

29

, also reported a nitrate-nitrite equilibrium on Cu-CHA catalysts by implementation of in situ FTIR, UV-vis and Cu Kedge XAS approaches.

Generally, the SCR reaction is sub-divided into standard SCR, which is the formation of nitrogen from NO and NH 3 without NO 2 , and fast SCR, which happens in the presence of NO 2 30 . A consequence of the NH 3 -SCR reaction scheme proposed by Janssens et al., 23 assumes that all intermediates in fast SCR are also part of the standard SCR cycle. Moreover, the activation energy obtained by DFT The variety of different active Fe-sites in the Fe-exchanged zeolites is even higher assuming also a possible formation of iron oxide cluster detected by UV-vis and FTIR spectroscopies in several works 33-38 . The formation of monomeric and dimeric iron species in Fe-ZSM-5 catalyst under different pretreatment conditions have been discussed on the basis of Fe Kedge EXAFS analysis In the same work the authors revealed reversible redox process occurring on the iron sites in Fe-BEA with 0.99 wt. % of Fe treated under nitrogen using operando Fe K-edge XANES. Earlier, the redox dynamics of Fe sites has been also investigated by EPR and optical spectroscopy 37, 38 . Also, numbers of studies have been done to investigate Fe-ZSM-5 catalysts by means of XAS proposing that the active sites are represented by di-nuclear iron oxo-/hydroxo cluster or an oligomeric iron-oxo species 42-45 . In the present work the Cu-CZC and Fe-MOR monometallic catalysts were selected for a XAS operando study due to their superior de-NO x activity respectively at low and hightemperatures, as shown in our previous work 22 . Both Cu-and Fe-speciation in monometallic catalysts and their mechanical mixture were investigated by means of XANES and EXAFS analysis. Particular attention has been given to Cu-speciation in the mixed system, since it demonstrated very different behavior with respect to the monometallic counterpart. The formation of different mobile and framework-interacting Cu species under NH 3 -SCR conditions has been quantitatively analyzed through principal component analysis (including advances statistical analysis) and further linear combination fit. Several hypotheses intended to explain the catalytic results and the mechanisms of the different Cu-speciation behavior in the monometallic and mixed catalysts have been proposed and critically discussed relying on the previously reported studies of SCR mechanism and ion migration processes in zeolites.

Experimental

Materials description and methods

Please do not adjust margins

Please do not adjust margins Protonated and copper exchanged silicoaluminophosphates (SAPO-34), CHA-type zeolites, were directly used as received from Clariant company. Commercial Mordenite (Si/Al = 6.2, Na + form) was received from Zeolyst.

The Fe-containing mordenite, abbreviated as Fe-MOR, was prepared by the conventional ion exchange procedure

22

. In the first step, 1 g of parent MOR was mixed with 40 mL of aqueous solutions containing 0.05 M of Fe(NO 3 ) 3 •9H 2 O stirred at T = 60 °C for 4 h. The obtained suspensions were centrifuged, washed thoroughly with deionized water, freezedried for 2 nights and then calcined at 500°C for 4 h. The ionexchange procedure was repeated three times. The metal exchanged forms of monometallic zeolites are further abbreviated as Cu-CZC and Fe-MOR. Despite of the fact that typically Al-substituted CHA (i.e. SSZ-13) demonstrates better hydrothermal stability than Cu-SAPO-34 (Cu-CZC), stability of the latter can be significantly enhanced for the materials with smaller crystallite size and low Cu concentration on the crystal surface 46 . On the other hand, utilization of Fe-MOR is motivated by the fact that Fe-MOR effectively eliminates N 2 O and exhibits high activity and excellent stability under practical conditions of NH 3 -assisted SCR.

The sample of bimetallic catalyst, containing both Cu-and Fe-exchanged zeolite has been prepared by a simple mechanical mixing of two equal fractions of the abovementioned components (0.5Cu-CZC + 0.5Fe-MOR) and further abbreviated as Cu-Fe-mix sample. The mixture was meticulously grounded in chemical mortar to promote a better mixing and close contact between the different zeolite grains.

The objects investigated in the present work through operando XAS experiment were previously exhaustively characterized by laboratory in situ FTIR as well as UV-vis spectroscopies 22 . Specific surface area was analyzed by BET technique performed within an ASAP 2020 MP analyzer. N 2 adsorption/desorption isotherms were collected at 77 K. The samples were degassed in situ at 350 o C for 3h prior to the measurements. The precise chemical composition of the samples was analyzed by ICP (Inductively Coupled Plasma) analysis. The Varian ICP-OES 720-ES spectrometer was employed to determine the contents of Si, Al, Cu and Fe in the samples.

XAS operando experiment details

Cu and Fe K-edge X-ray absorption near-edge structure (XANES) and extended X-ray absorption fines structure (EXAFS) spectra were measured at BM23 beamline of the European Synchrotron Radiation Facility (ESRF, Grenoble, France) 47 . A Si(111) double-crystal monochromator was used for energy scanning, whereas harmonics rejection was done by two flat Si mirrors positioned at 2.8 mrad. Incident and transmitted X-ray intensities were measured by three ionization chambers with gas filling acceptable for both Fe and Cu K-edges. The spectrum of Cu or Fe foil was collected simultaneously with each spectrum of the sample at the corresponding edge to ensure the energy calibration. XAS data reduction and XANES linear combination analysis were carried out in Athena, whereas EXAFS fitting was done in Artemis, both codes being part of Demeter package 48 .

The powdered samples of monometallic catalysts have been prepared in the form of self-supporting pellets with the mass optimized for optimal signal-to-noise ratio that were computed within XAFSmass code 49 . The optimal mass for Cu-CZC is 109.3 mg, while for high-loaded Fe-MOR the optimal adsorption step could be achieved for the pellet mass of 38 mg. For mechanical mixture (Cu-Fe-mix), the optimized mass equal to 86.5 mg (43.25 mg for each component) was utilized as compromise in order to get appropriate absorption step both for Cu-and Fe-K-edges. The pellets were fixed inside the Aabspec CXX (ultra-low volume flow-through) reactor cell, initially dedicated to operando IR measurements and further customized for operando XAS measurements by substituting the standard KBr windows by Kapton ones. The cell belongs to the class of ultra-low volume flow-through cells that are very suitable for catalytic experiments.

The SCR experiment has been designed to carry out the same reaction under synchrotron beam and in a laboratory, by using the same Aabspec CXX 800 o C reactor-cell. The activation was performed by heating the samples from RT to 500 ℃ under 10 % O 2 /He flow with a ramp rate of 5 ℃/min. Cu and/or Fe K-edge EXAFS data were collected at 200 ℃ and at 500 ℃ (ca. 20 min/scan). After the activation, EXAFS spectra were measured at fixed temperatures in the range from 450 °C to 150 °C with the step of 50 °C under the NH 3 -SCR conditions: 500 ppm NO, 500 ppm NH 3 , 10% O 2 , 2% H 2 O balanced in He, with 100 ml/min total flow rate. The gas flow composition has been slightly simplified with respect to those used in laboratory experiment. The detailed description of the catalytic experiment in the lab is given in Section 1 of SI. The temperature ramp both upon the activation and transitions between the temperature points in SCR conditions were followed by faster XANES acquisitions (ca. 7 min/scan). For each temperature point along SCR ramp the EXAFS spectra have been taken for steady-state conditions after the stabilization of the system continuously monitored by XANES.

Importantly, Fe and Cu K-edge spectra for the mixed bimetallic sample were collected in a single run using the same pellet (thus making the dwell time at each temperature point roughly twice as long compared to the single-metal samples). Catalytic activity of the samples was evaluated simultaneously with XAS data acquisition by monitoring the effluent gas composition by an online mass spectrometer (Balzers Prisma). Activity of the samples was calculated using the NO signal (m/z = 30) corrected for MS drift using He signal (m/z = 4). The conversion data are reported in Section 3.2. Reported values were calculated as a difference between the outlet and inlet MS signal, preliminary normalized by He signal level: Please do not adjust margins

Results

Preliminary characterization

Please do not adjust margins

The physicochemical properties of the monometallic Cu-CZC and Fe-MOR catalysts and corresponding parent notexchanged zeolites were first investigated using XRD, N 2 physisorption at 77 K, ICP and FTIR in-situ spectroscopies. The results are summarized in Table 1.

The ICP analysis shows that the copper and iron contents are about 1.56 wt. % of Cu and 7.55 wt. % of Fe for Cu-CZC and Fe-MOR samples, respectively. Corresponding (P+Al):Si and Cu/Si molar ratios are 11.2 and 0.44, respectively. The Si/Al molar ratio slightly increase after iron exchange of MOR framework, indicating a moderate decrease of framework Al content.

The PXRD patterns of the parent and metal exchanged zeolites are shown in Figure S2 of SI. It confirms that chabazite and mordenite crystal structures are maintained well after metal exchange. Only slight decrease in the reflection intensity was observed for Fe-MOR. This result can be related to the partial loss of framework crystallinity and to the absorption of X-rays by inserted metal ions, especially for high-loading Fe-MOR (See FigureS2 of SI). It should be noted that no traces of M x O y (M = Cu, Fe) oxide or metallic phases were detected in Cu-CZC and Fe-MOR patterns, suggesting that the metal species exist in highly dispersed states or they form some very small clusters that are beyond the detection limit of laboratory PXRD.

The BET surface area of Cu-CZC and Fe-MOR sample is around 568 m 2 /g and 483 m 2 /g, respectively. The iron loading in MOR structure causes a slight increase in BET surface areas and micro porosity likely due to the elimination of residual impurities in MOR micropores during washing steps. The total acidity and density of Lewis and Brønsted acid sites in the investigated catalysts has been determined by in situ FTIR after exposure to pyridine as reported in our previous study

22

. The data confirmed that copper remained a marginal Brønsted acidity in the Cu-CZC sample (0.11 μmole/g) with an additional Lewis acidity (17.8 μmol/g). The later remained accountable on Cu-CZC after desorption beyond 150 °C, indicating the presence of strong acidic sites in this sample. The concentration of Lewis acid sites was 64.7 μmol/g for Fe-MOR. An increased in the Lewis acidity took place when the temperature increased from 100 to 350 °C over Fe-MOR, suggesting that some Lewis acid sites of medium-high strength could be recovered during the thermo-decomposition of pyridine *as obtained from ICP analysis

Catalytic performance

This journal is © The Royal Society of Chemistry 20xx J. Name., 2013, 00, 1-3 | 5

Please do not adjust margins

Please do not adjust margins

The catalytic activity of the samples was monitored upon operando XAS experiment by online MS spectrometry as described in Section 2.2. NO conversion data measured upon operando XAS experiment are reported in Figure Erreur ! Source du renvoi introuvable.(a). Because of the differences in experimental conditions with respect to the previously reported laboratory results for the investigated samples Aiming to shed light on the origin of such catalytic properties, we investigated Cu and Fe speciation in the single-component Cu-CZC, Fe-MOR and their mechanical mixture during activation and under reaction conditions by X-ray absorption spectroscopy. C in comparison with the data collected on the iron oxide α-Fe(III) 2 O 3 (hematite phase). The features around the main threshold of XANES spectrum are associated with 1s4p dipole transitions, while the small peak in the pre-edge region is assigned to transitions from 1s to 3d-4p hybridized states caused by noncentrosymmetry of the Fe species, as well as to quadrupole (dipole forbidden) 1s3d transitions 50, 51 .

Fe-speciation upon activation and SCR

The results show that the Fe K-edge XANES spectra of the mixture at RT exhibit a very similar shape to α-Fe 2 O 3 oxide, and thus probably Fe species in the investigated sample have very similar local atomic environment, to the one observed for the Please do not adjust margins Please do not adjust margins bulk α-Fe 2 O 3 oxide (hematite). However, since no traces of this oxide phase were detected by PXRD, most of the iron atoms likely form very small Fe-O atomic clusters. The activation process is accompanied by a small gradual decrease of the main maximum intensity as well as an energy shift of the absorption threshold towards the lower energy, reflecting some weak temperature-induced structural rearrangements upon activation. The inset of Figure 2 shows magnified background subtracted pre-edge peak intensity along the activation process. The intensity of the pre-edge peak increases with heating from RT to 500 °C, thus indicating an increase of the abundance of Fe-sites in T h coordination as it was suggested in for Fe-MOR with different Fe loading 52 . Fe K-edge XANES collected for Fe-MOR upon sample demonstrate very similar trends and do not reported here for brevity.

A further structural refinement of the small Fe-O clusters suggested to be formed both in monometallic Fe-MOR and Cu-Fe-mixed samples, was performed by means Fe K-edge EXAFS Fourier analysis. The k The temperature evolution of the FT-EXAFS amplitudes collected on Cu-Fe-mixed sample during activation and SCR conditions is accompanied by the gradual damping of the FT-EXAFS signal. Qualitatively the observed trends assume almost no changes in the average local atomic structure in the proximity of iron sites upon activation (See Figure 3, top) and under SCR conditions (See Figure 3, bottom), while the decrease of the intensity upon temperature increase under SCR is related with the temperature effect on the EXAFS signal.

To get quantitative estimation of the changes observed between the samples and α-Fe 2 O 3 bulk oxide as well as changes caused by temperature-driven evolution upon activation, the EXAFS fit was performed. Due to the similarities in the localization of the peaks as well as overall similarity of EXAFS amplitudes obtained for investigated samples and α-Fe 2 O 3 54 (American Mineralogist database, str. № 0000143), the latter has been used as an initial guess for the fit. To emphasize a different behaviour of the first and higher coordination shells, we have performed EXAFS-analysis in the R-range from 1.1 to 3.5 Å, thus capturing the 2 nd and 3 rd peaks of experimental FT-EXAFS amplitudes. All SS and MS paths contributions within the effective path lengths up to 4.2 Å have been accounted for the fit. Different SS and MS paths were parameterized by scaling coefficients n1, n2 and n3 intended to describe CNs of the first (n1) and higher coordination shells (n2, n3). More details on EXAFS fit parametrization are reported in SI. First, EXAFS fit of the experimental data collected on bulk iron oxide α-Fe 2 O 3 was performed in order to get reliable value for passive amplitude reduction factor S 0 2 , that was further fixed for all subsequent fits. In spite of the well-defined structural parameters of model compound (α-Fe 2 O 3 ) the coordination numbers (i.e. n1, n2, n3 coeff.) and displacement parameters R i have been set as fit parameters to provide more reliable structural parameters refinement for the investigated catalysts. The fit results for oxide phase, Fe-MOR and Cu-Fe-mix samples at RT (before the activation) are reported in Table 2.

Table 2. The fit results reported for Fe K-edge k 2 -weighted FT-EXAFS amplitudes obtained for bulk oxide phase α-Fe2O3 as well as Fe-MOR and Cu-Fe-mix catalysts at RT. The variables that have been fixed upon fit procedure are underlined. *an averaged cluster diameter <D> was estimated by using Calvin's mode 55,56 Unlike the case of first oxygen shells characterized by the very similar CNs (i.e. similar values for n1 scaling coefficient) both for α-Fe 2 O 3 and investigated asmples, a great discrepancy for n2 and n3 CNs scaling coefficients was obtained (See Table 2 and Figure S3 of SI). EXAFS fit yields significantly lower n2 and n3 values for Cu-Fe-mix sample reflecting a drastic decrease of the CNs for higher coordination shells. This reduction of CNs is clearly caused by the small size of Fe 2 O 3 oxide clusters formed in both samples. Along with CNs reduction the small decrease in the distances by ⁓ 0.01 Å and ⁓ 0.02 Å (See Table 2), obtained for the first two oxygen subshells, supports the idea of small cluster size. DW factors obtained for Cu-Fe-mix and Fe-MOR samples are significantly higher with respect to those refined for α-Fe 2 O 3 , reflecting significantly higher disorder in local atomic structure of Fe-O clusters formed in the catalyst. Nevertheless, the good fit quality (R-factor = 0.0025 and 0.0029 for Cu-Fe-mix and Fe-MOR RT dataset, respectively) confirms that local atomic structure of small Fe-O clusters is very similar to the shortrange atomic order in bulk hematite α-Fe 2 O 3 . The obtained result in a good agreement with those reported in ref 57 , where the formation of hematite NPs in highly loaded Fe-BEA (5.1 wt. % of Fe) was revealed by UV-vis and EXAFS analysis.

Afterwards the experimental FT-EXAFS amplitudes collected for Cu-Fe-mixed sample at 200 o C and 500 o C were analyzed with a fixed scaling coefficients n1, n2, n3 as obtained for RT fit. As expected, higher temperature EXAFS fits characterized by further essential increase of DW factors, providing a good fit quality reflected in very small R-factors both for 200 o C and 500 o C (0.003 and 0.004, respectively; See Table S3 of SI). The same trend is observed for the EXAFS fit of the data collected under SCR condition -the difference observed in the signal might be reliably associated mostly with temperature effect (See Table S3 and Figure S4 of SI).

Since no traces of iron oxide phases have been found in PXRD patterns acquired for single-component Fe-MOR sample (See Figure S2 of SI) the size of the Fe-O clusters is supposed to be less than laboratory X-ray diffractometer detection limit. To estimate the size of Fe-O clusters formed in the catalysts we have parametrized CNs in accordance with Calvin's model accounting for averaged particle size (roughly assuming for a spherical shape of the cluster) as described elsewhere 55, 56 :

where N i is the coordination numbers of i-scattering path (in cluster and in bulk materials, in accordance with the upper index), R i -is the effective path lengths (in Å), D is the mean cluster diameter (in Å). This approach yields an averaged cluster's size to be equal to 2.24±0.75 nm for the Cu-Fe-mixed catalyst and even slightly lower (2.20±0.73 nm) for monometallic Fe-MOR (See Table S2 of SI). The fit results obtained by means Calvin's model (i.e. eq. 2) is reported in Figure S3 of SI.

In fact, in case of broad distribution of the particle size this approach results in the size weighted toward the low part of the distribution 55 ; thus the real averaged size of the clusters could be slightly larger and it implies that most of the Fe-O clusters are likely formed on the exterior surface of MOR crystals. This is in line with BET analysis, since even for highly loaded Fe-MOR the decrease in specific surface area after ionexchange were not observed (See Table 1), suggesting that no relatively big Fe agglomerates are formed inside MOR cavities.

To sum up, above described results obtained on the basis of XANES and EXAFS analysis declare that most of the Fe atomic species in the both catalysts are involved in the formation of very small iron clusters with local atomic structure similar to α-Fe 2 O 3 oxide phase. However, analysis of the differential XANES signal reported in Figure S5 of SI allow to catch some tiny differences in Fe speciation. Taking into account that no appreciable structural differences was declared by means of EXAFS fit for high and low temperature datasets, the changes observed by differential XANES could be associated with the trace of minority of the isolated Fespecies.

Particularly the decrease of differential XANES signal observed for high temperature data (T > 350 o C) could be associated with the involvement of isolated Fe sites into redox chemistry at high temperature. Indeed, for previously reported catalytic activity for Fe-exchanged zeolites with moderate Me-loading (that is not implying a favorable condition for Fe clusterization), the onset of de-NO x activity is observed at 300-400 o C 9, 12, 36 . This fact reinforces our hypothesis about minority of isolated Fe-species that are likely involved in redox chemistry at higher temperature forming similar intermediates. This would result to the same averaged oxidation state and coordination environment of isolated Fe sites, thus damping differential XANES signal. It can be explained by the formation of some ammonia or water solvated iron complexes at high T under SCR conditions or due to hydrothermal aging 58, 59 .

The results of differential XANES analysis are supported by the findings of statistical and PCA (Principal Component Analysis) analysis performed on Fe K-edge dataset. Importantly, the abstract components derived by using statistical analysis implemented in PyFitit package 60 closely This journal is © The Royal Society of Chemistry 20xx

Please do not adjust margins Please do not adjust margins resemble the differential XANES obtained for temperature induced evolution in Fe-MOR and the one obtained as a differential signal between Fe-MOR and Cu-Fe-mix samples after high-temperature O 2 -activation (See Figure S9 of SI). Thus, differential XANES signal can be more reliably associated with the presence of minority of the isolated Fe-sites in the catalysts. However, the good quality of the EXAFS fit obtained on the basis of distorted α-Fe 2 O 3 structure assume very low relative abundancy of the isolated Fe-sites, that is in a good agreement with very low dispersion (4%) of the isolated Fesites obtained by IR 22 .

Summarizing . This likely results in lack of ammonia coordinated Cu I complexes at high temperature under SCR conditions in the mixed catalyst as discussed in next section. The latter can suppress the activity of Cu-exchanged component in the high temperature SCR, but at the same time it should yield an improvement in N 2 O selectivity of Cu-Fe-mix catalyst at high temperature region.

Cu-speciation upon activation and SCR

Cu K-edge XANES spectra consist of several distinct features indicative of the various electronic transitions for the Cu(I) and Cu(II) cations 62 . The peaks located at around 8977.0 eV and 8987.0 eV are representative of Cu(II) species. The first one is originated from the dipole-forbidden 1s3d transition, which becomes allowed due to mixing of the 3d and 4p orbitals and has been reported in several studies as a low intensity pre-edge feature 63, 64 . The shoulder at 8987.0 eV is due to the 1s4p electronic transition in Cu(II). The presence of the feature centered around 8983.0 eV is characteristic of the 1s4p transition for a Cu(I) two-coordinated complexes in almost linear geometry (hereinafter referred to as Cu(I) risingedge feature) Please do not adjust margins Please do not adjust margins As it was discussed above, the activated state of the Cu-CZC and Cu-Fe-mix samples yields very similar XANES and EXAFS signals (See Figure S12 of SI), declaring no significant changes in Cu-speciation upon high-temperature pretreatment. Also, the evolution of the XANES spectra obtained for monometallic Cu-CZC sample under SCR conditions (as reported in a previous section) is in good agreement with previously reported data for Cu-SAPO-34 45 . However, rather different Cu-speciation has been observed under reaction conditions for bimetallic Cu-Fe-mixed sample comparing to Cu-CZC for the whole temperature range, as shown in XANES and FT-EXAFS amplitudes reported on Figure 6. One observes that the most explicit differences between monometallic Cu-CZC and bimetallic Cu-Fe-mix samples reflected in the different intensity of Cu(I) rising edge feature (located at ca. 8983.0 eV) as well as in the different intensity and shape of WL peak in the XANES part of the spectra (See Figure 6a).

Indeed, for the high temperature data collected at 450 o C

(under NH 3 -SCR conditions) Cu sites in Cu-CZC sample are notably more reduced with respect to Cu-Fe-mix sample. However, the situation drastically changes for temperatures below 300 o C, where the maximum of Cu(I) rising-edge intensity is observed for Cu-CZC (being already less developed compared to Cu-Fe-mix sample). For Cu-Fe-mix the 1s4p Cu(I) rising-edge feature grows with the decrease of temperature (See Figure 6a), reaching maximum at 200 ℃ and revealing significant reduction of Cu-sites. At 150 ℃ it remains to be well developed for Cu-Fe-mixed sample (the intensity of this feature is still much higher than at 300 ℃, in contrast with Cu-CZC case).

Even at 100 ℃ in the Cu(I) rising-edge region one could observe well-developed step-like shoulder for Cu-Fe-mixed sample, while it almost disappears for monometallic Cu-CZC.

In the EXAFS parts (See Figure 6b) at higher temperature range one clearly observes 2nd shell maxima both for Cu-CZC and Cu-Fe-mix samples which is, accordingly to the previously reported EXAFS findings 25 , associated with the formation of framework coordinated Cu-oxo species Z-Cu II (OH)/O 2 and nitrate species such as Z-Cu II (NO 3 ). In addition to the different abundancy of reduced mobile Cu(I) amino-complexes (proved by XANES), that obviously results in different intensity of the 1st shell maximum in FT-EXAFS signal (due to the lower coordination number for mobile di-amino complexes, CN=2), the most conspicuous difference observed for the temperature evolution of FT-EXAFS signal under SCR conditions lies in the 2 nd shell peak intensity evolution at the middle temperature range. Indeed, one can emphasize not negligible contribution to the 2 nd shell maximum still observed for Cu-CZC at 250 ℃, whereas the signal obtained for Cu-Femixed catalysts in this region lacks of intensity. As it was mentioned above, the quantitative EXAFS analysis is complicated because of the big variety of different Cu species that could be formed and contribute to the averaged EXAFS signal under reaction conditions 28, 70 .

Quantification of Cu-species under reaction conditions

In this section, the relative abundancy of the different Cuspecies is quantified under reaction conditions using XANES LCF (Linear Combination Fit) analysis. Based on the previously , five principal components were used in order to reproduce each spectrum from the entire dataset. The details on statistical and PCA analysis as well as motivation for the selected reference spectra for LCF analysis are reported in Supporting Information. The results of LCF analysis are reported at Figure 7 (a-b). For the sake of simplicity, the contribution from two different framework coordinated complexes (Z-Cu

Discussion

Overall, the temperature-driven behavior of different pure components demonstrates significantly higher abundancy of the mobile linear di-amino complexes at the low and medium temperature SCR for Cu-Fe-mixed catalyst with respect to pure copper catalyst Cu-CZC (See Figure 7a,b).

Figure 7c represents conversion data collected upon the XAS operando experiment obtained by monitoring NO traces using MS spectrometry. MS data evidently demonstrate lower NO conversion for Cu-Fe-mixed sample in the low temperature range (T < 250 A direct interaction between Cu and Fe gas sites or the formation of any Cu-Fe conglomerates is excluded because no Cu-Fe interactions were evidenced by XANES or EXAFS analysis, both for Cu and Fe K-edges. The possible explanation of the different Cu-speciation is based on the fact that lower conversion observed for mechanical mixture may result in the scenario when Cu sites in Cu-Fe-mixed catalyst in average are exposed to the gas feed that contains more reactant molecules (namely, NH 3 and NO), with respect to the case of monometallic Cu-CZC catalyst. Such conditions are likely to be favourable for the higher reducibility of the Cu sites observed for the mixed catalyst. Indeed, recently Doronkin et al. 45 have

shown the evolution of the Cu oxidation state along a capillary (by operando Cu K-edge XANES) at the fixed temperature and gas feed composition, exhibiting higher abundancy of Cu II sites at downstream end of the capillary, where the copper ions are exposed to lean SCR gas mixture. Apparently, when the highly productive at low temperature region Cu-CZC catalyst is diluted by less active Fe-MOR counterpart an averaged oxidation state of Cu in the pellet can decrease, similarly to the capillary case described by Doronkin et al. 45 .

Besides, low-temperature SCR mechanism recently proposed in the literature 31, 32 76 may contribute to the observed effect as well. It has been shown that a re-oxidation cycle at low temperature SCR may occur by the activation of oxygen through the dimerization reaction of two proximal mobile di-amino complexes 31, 32, 76 , implying a pseudohomogeneous character of the reaction. and NO molecules in a feed facilitate SSIE independently on the primary source of copper, i.e. Cu(I) or Cu(II) oxides [79][80][81] .

In line with the above described SSEI migration mechanism, we can hypothesize that when Cu-CZC catalyst diluted by Fe-MOR counterpart, some fraction of NH 3 -solvated di-amino complexes can gradually migrate from the SAPO-34 to MOR framework environment under SCR condition in low-medium temperature range -passing through the interface between different zeolite grains. This assumption is in good agreement with very recent work by H. Lee et al., 82 , where inter-particle Cu migration were investigated for Cu-exchanged and protonated SSZ-13 prepared by simple mechanical mixing. It was shown that after hydrothermal aging the mixture of Cu-SSZ-13 and H-SSZ-13 behaves in a very similar way as Cu-SSZ-13 with two times lower Cu-content, assuming almost homogeneous distribution of Cu in the mixture. The SSEI and Cu migration upon hydrothermal aging for Cu-SAPO-34 are also reported elsewhere 83-85 .

In our case the proposed migration phenomenon will gradually decrease the density of Cu I (NH 3 ) 2 species in Cu-Femix sample (with respect to those for monometallic copper zeolite) and increase the number of "uncoupled" di-amino complexes in mechanical mixture. It should eventually inhibit the oxygen activation via dimerization reaction and thus prevent re-oxidation of Cu I Cu II . Thus, the migration mechanism can be one of the reasons of higher abundance of reduced Cu I sites in the Cu-Fe-mix sample below 250 o C (as reported in Figure 7(a-b), where the major part of Cu(I) component is represented by mobile Cu I (NH 3 ) 2 complexes. This higher abundance of reduced Cu I sites might be also considered as a consequence of decreased efficiency in the oxidation of NO into NO 2 (only NO is fed and only NO 2 traces were detected in parallel laboratory IR experiment), which hinders the fast SCR reaction, so degrading the catalyst performance respect to the case when equimolar amounts of NO and NO 2 are fed among reactants. With respect to the previously published results

22

, some apparent discrepancies need to be addressed. First, the clear synergetic effects of the physical mixture appear less clear in the present work. There are a number of reasons for this.

First, in this work the catalysts systems are compared under standard SCR conditions, while fast SCR conditions were applied in 22 , i.e. we use only NO, and not NO 2 . In this work we observe depletion of the Cu concentration in Cu-CZC counterpart because of the Cu migration in the physical mixture. This mitigates especially the low temperature reoxidation, which in turn is not affected to the same degree under fast SCR conditions. Second, the different catalyst loadings employed due to the optimization of the XAS signals makes the comparative kinetic analysis more complex. In order to clarify this we have made a simple elaboration of the kinetic analysis based on pseudo first order derived kinetic constants, and thus compared the performance of the systems at GHSV 50.000 h -1 to exhibit the behavior under realistic conditions (See Figure Erreur ! Source du renvoi introuvable.). What is seen is that some synergetic effects are observed (See Figure Erreur ! Source du renvoi introuvable.), but they are less pronounced due to the use of standard SCR gas conditions and dampened due to the observed Cu migration.

Summarizing, we observe that the dilution of the monometallic Cu-CZC catalyst by the mixing with Fe-MOR (lowactive towards NO conversion at the low-temperature SCR) results to the higher reducibility of the Cu sites in middle and low temperature SCR observed by operando XAS experiment. The presence of the less active Fe-MOR can result in the gas feed in proximity of Cu-sites that has elevated concentration of NH 3 and NO. This will stimulate the migration process of NH 3solvated mobile di-amino complexes from Cu-CZC to large pores Fe-MOR.

This copper migration eventually decreases the spatial density of mobile Cu I complexes in the entire system, thus inhibiting the dimerization reaction -considered as a key step for the re-oxidation cycle of low-temperature SCR. This would result in higher reducibility of the Cu sites in the mixed sample, clearly observed by Cu K-edge XAS. From the other side this ionic migration process may results to the redistribution of copper sites forming more effective catalytic phase in the zeolite framework that resulted in synergetic effect observed for the first time in 22 and partially inhibited here by the specific reaction condition. Furthermore, the detailed information derived from the XAS data in this study allows us to further suggest an optimization of such physical mixtures. In order to precompensate for the observed Cu loss due to migration, mixtures with less fraction of Fe-MOR and high fraction of Cu-CZC can be used (i.e. 70 % of Cu-CZC and 30 % of Fe-MOR). Note that the main synergetic effect and role of Fe-MOR is to be a high temperature, in proximity, NO x (N 2 O, NO, NO 2 ) scavenger preventing poor high temperature performance of high temperature unselective Cu-CZC. Above 300 Please do not adjust margins Please do not adjust margins are orders of magnitudes higher when selectivity is upheld as in the case of Fe-MOR (See Section S1 of SI). Thus, it would not be expected to be harmful for high temperature performance to use e.g. 30% Fe-MOR instead of 50% in the mixture that will be the subject of our further studies. In summary, the physical mixtures remain a very interesting and practical solution to achieve a complete temperature window for the SCR reaction, and this work helps understanding the precise speciation and thus provide future guidance to design of such systems.

Conclusions

The mechanical mixture (Cu-Fe-mixed), already showed superior activities than the monometallic exchanged zeolites, and it was prepared in a simple way by mixing Cu-exchanged (Cu-SAPO-34) and Fe-exchanged (Fe-MOR) catalysts. To understand the reason of this phenomenon, the monometallic and mixture catalysts were investigated by operando XAS spectroscopy under NH 3 -SCR conditions in a wide temperature range. It should be noted that the results obtained during the operando XAS experiment at the synchrotron were very reproducible at LCS laboratory under the same conditions.

The PXRD analysis evidences no traces of bulk metal oxides both in parent monometallic and mixed bimetallic catalysts. Fe K-edge XANES and EXAFS analysis shows that most of the iron species in Fe-MOR and Cu-Fe-mix samples exist in the form of small iron oxide cluster (beyond the limit of laboratory XRD) with a local atomic structure similar to bulky α-Fe 2 O 3 (hematite phase). The cluster size was estimated as ⁓ 2.3 ± 0.6 nm by means of EXAFS fitting. The changes in the Fe K-edge EXAFS spectra observed both upon high temperature activation and under SCR conditions at different temperatures are mostly due to the temperature effect without any significant structural modifications. However, differential Fe Kedge XANES reveals the involvement of minority of isolated iron sites into redox chemistry in the high temperature SCR.

Analysis of Cu K-edge dataset acquired upon high temperature O 2 -activation do not exhibit any significant changes between Cu-speciation in monometallic and bimetallic catalysts. However, dramatical differences were observed under reaction conditions, particularly in the low-temperature range. XANES LCF analysis clearly demonstrates that the presence of Fe-MOR component changes the Cu I :Cu II balance in the mechanical mixture declaring significantly higher abundance for mobile Cu I di-amino complexes in the low temperature range. The latter, in principle could be considered as a reason of such different behavior of Cu-speciation simply accounting for higher availability of the reactant molecules (i.e. NO and NH 3 molecules) in proximity of Cu sites for the Cu-Femixed sample. Additionally, the dilution of Cu-CZC catalyst by the large-pores Fe-MOR may initiate gradual migration of mobile Cu I complexes to MOR framework, similarly to SSIE mechanism, that will inhibit the oxygen activation via dimerization reaction (proposed as a key step for lowtemperature SCR), thus preventing the re-oxidation step and yielding higher reducibility of Cu sites in mechanical mixture clearly observed by XAS. This work generates clear suggestions on how to circumvent this for the design of future SCR solution based on physical mixtures.

This work is dedicated to the memory of Prof. Carlo Lamberti.

We will be always indebted to Carlo, for his constant support and brilliant guidance in the use of synchrotron ration to solve wide range of problems in catalysis. It is difficult to overestimate his contribution to the research dedicated to characterization of catalysts via in situ and operando synchrotron and laboratory experiments. We will always remember his unique enthusiasm in work and in everyday life

Notes and references

22 , 1 ) 36 , 22 ,

 2213622 we have repeated catalytic experiment in the lab using the mass of the catalysts and total flow rate similar to those employed during operando XAS experiment. Corresponding data are reported as dashed curves in Figure Erreur ! Source du renvoi introuvable.. One can notice an excellent agreement between conversion rates obtained during the operando XAS experiment at the synchrotron and those re-measured in the lab. Moreover, since weights of the catalysts were optimized in order to have the best XAS signal above both Cu and Fe K-edges we introduced additional corrections. Figure Erreur ! Source du renvoi introuvable.(b) reports corrected NO conversion data for the two catalytic experiments that account for different catalysts mass and relevant reaction condition (i.e. GHSV = 50 000 h -, as detailed in Section 1 of SI. One can see that Cu-Fe-fix sample prepared as simple mechanical mixture of Cu-and Fe-exchanged zeolites represents a compromise solution being highly effective at both low and high temperature SCR. Indeed, from Figure Erreur ! Source du renvoi introuvable.(b) it is clear that in the low temperature range the conversion rate observed for mechanical mixture is competitive with those obtained for one-component Cu-CZC catalyst. Furthermore, as it was shown by Gao and co-workers, the presence of Fe-exchanged component may lead to decrease in N 2 O release 12, improving the selectivity of mixed catalysts in high temperature range with respect to one-component Cu-CZC catalyst.However, it should be noted that a nearly 100 % selectivity for all the studied samples was observed in our recently published laboratory experiments in particular no N 2 O was detected. That agrees well with the linear dependence of N 2 vs NO conversion observed for all 3 catalysts in the current operando XAS study (See FigureS1of SI).

Figure

  Figure Erreur ! Source du renvoi introuvable.(c) shows the experimental NO conversion curves recalculated using the kinetic constants averaged over the two experiments (operando XAS and laboratory ones) in comparison with the theoretical curve simulated for the mixed material for the case when its Cu-CZC and Fe-MOR components work independently. One can clearly observe that at 200 o C the experimental catalytic activity obtained for Cu-Fe-mix sample exceeds the conversion rate expected from the mixture of non-interacting components. This observation is in line with the synergetic effect observed for Cu-Fe-mix sample in our previous work 22 .

Figure 2

 2 Figure 2 reports Fe K-edge XANES spectra collected for Cu-Fe-mixed sample under steady state conditions upon the activation in air at RT, 200 o C and 500 o

Figure 1 (

 1 Figure 1 (a) NO conversion measured for Cu-CZC, Fe-MOR and their mechanical mixture during operando XAS experiment and in the lab with similar mass of the catalyst pellets and total flux. (b) NO conversion data recalculated for relevant reaction conditions (GHSV = 50 000 h -1 ) as detailed in Section 1 of SI (c) Experimental NO conversion curves recalculated using the kinetic constants averaged over operando XAS and laboratory experiments together with the theoretical curve (green curve) simulated for the mixed material for the case when its Cu-CZC and Fe-MOR components work independently

Fig. 2

 2 Fig. 2 Fe K-edge XANES spectra collected for Cu-Fe-mixed sample under steady-state conditions at RT, 200 o C and 500 o C upon the activation in oxygen in comparison with the data collected on the bulky iron oxide α-Fe(III)2O3 shown as a dashed curve. The inset show magnification of background subtracted pre-edge peak.

2 -

 2 weighted FT-EXAFS amplitudes obtained for Cu-Fe-mixed sample upon activation process under steady state conditions at RT, 200 o C and 500 o C are reported in Figure 3 (top part), while the temperature evolution of the EXAFS signal upon NH 3 -SCR condition reported in Figure 3 (bottom part). The qualitative examination show that the main features in EXAFS amplitudes obtained for Cu-Fe-mixed sample upon activation correspond to α-Fe 2 O 3 bulk oxide phase. The intensity of the 1 st coordination shell maximum (denoted as peak A at Figure 3, top) obtained for the catalyst at RT is slightly lower compared to α-Fe 2 O 3 . However, significantly more essential decrease of the 2 nd and 3 rd FT-EXAFS maxima intensity (denoted as peak B and C at Figure 3, top) can be observed. This could be associated with the size effect for a small Fe-O clusters formed in the catalyst. Indeed, significantly more damped oscillation in the extended post-edge region of the normalized XANES signal (See Figure S17 of SI) confirms strong particle size-effect.

Fig. 3

 3 Fig.3Fe K-edge Fourier transformed phase uncorrected amplitudes of k 2weighted experimental EXAFS signal collected for bimetallic Cu-Fe-mix in comparison with the data collected at ambient conditions for bulk α-Fe 2 O 3 phase: upon high temperature O2-activation (top part) and under NH3-SCR reaction condition in a wide temperature range (bottom part). The vertical dashed lines correspond to the peak positions for α-Fe2O3.

.

  The Cu K-edge XANES spectra collected in steady state condition upon activation in oxygen (gas feed 10% O 2 + 90% He) are reported in Figure 4. The gradual heating up to 200 o C results in the formation of Cu(I)/Cu(II) rising-edge shoulders. The developments of Cu(I) rising-edge feature is continued with the further temperature increase reaching a maximum at around ⁓ 400 о C (See Figure S15 of SI for more detailed Tdriven evolution of Cu K-edge XANES upon activation). Afterwards the intensity of Cu(I) rising edge shoulder starts to decrease denoting re-oxidation phase. XANES spectrum obtained for the O 2 -activated Cu-CZC sample closely resemble the one recently reported by Kvande et. al. 65 for Cu-SAPO-34 with a very similar Cu loading and lower Si content (1.58 wt% Cu, Cu:Si = 0.25).

Fig. 4 74 . 5 .

 4745 Fig. 4 Cu K-edge XANES spectra collected for monometallic Cu-CZC catalysts under steady-state conditions at RT, 200 o C and 500 o C upon the activation in oxygen. Vertical dashed lines corresponds to the position rising-edge features assotiated with 1s4p transition in CuI (A) or CuII/CuI (B) configurations.In accordance with the literature 25, 26, 66, 67 , the Cu K-edge XANES collected both for monometallic Cu-CZC and mixed samples in hydrated state closely resemble those collected on a Cu(II)-acetate aqueous solution and hydrated Cu-exchanged Cu-SSZ-13 sample. Considering structural similarity of SAPO-34 and SSZ-13 frameworks, both monometallic Cu-CZC and Cu-Femix samples undergo several stages upon high-temperature activation in oxygen: (i) dehydration (accompanied by drastic decrease in the intensity of WL peak and simultaneous developing of Cu(I) and Cu(I)/Cu(II) rising-edge features, denoted as feature A and B in Figure 4 (ii) transient reduction (characterized by gradual decrease of the WL peak intensity and maxima for Cu(I) rising-edge feature) followed by (iii) Reoxidation (associated with notable loss of feature A intensity and minor restoration of WL peak intensity, see Figure S15 of SI). The stage (ii) takes place even in the abundant presence of oxidative agent such as oxygen 68, 69 . Considering previous works 25, 70-73 the final state in O 2activated catalyst (See red curve in Figure 4) can be assigned to different framework-coordinated Cu-sites dominated by Cu II

Fig. 5 75 Fig. 6 (

 5756 Fig. 5 Cu K-edge XANES spectra collected for monometallic Cu-CZC sample under steady-state NH3-SCR reaction conditions at different temperatures.The inset demonstrates corresponding k 2 -weighted phase uncorrected FT-EXAFS amplitudes.The spectra collected in the middle temperature range (i.e. 250 o C/300 o C) for Cu-CZC sample investigated in the present work (ca. 1.56 wt. % Cu, and Cu:Si ratio 0.44) demonstrate very similar XANES signal as reported for Cu-SAPO-34 (3.48 wt % Cu) by Doronkin et al. 45 . One observes raise of the characteristic Cu(I) rising-edge feature (located at ca. 8983.0 eV) with a temperature decrease that is reaching a maximum at 300 o C. Afterwards it starts to drop down with further temperature decrease down to 150 o C. At low temperature range a significant increase of the WL peak intensity is observed due to approaching of the favorable conditions for re-hydration of the sample by water molecules present in the reaction feed. At 100 o C Cu-CZC sample is partially re-hydrated but a very weak contribution in the region of Cu(I) rising-edge feature remains in the spectra.The temperature-driven behaviors of single-component Cu-CZC catalysts are in a good agreement with the previous studies on Cu-SSZ-13 catalyst 23, 28, 70 . In these studies, the development of Cu(I) rising-edge feature has been assigned to the formation of mobile linear di-amino complexes. Moreover, the lack of the intensity in the second shell region observed in EXAFS signal at low temperature range has been explained by the formation of ammonia solvated mobile complexes, including tetra-amino complexes23 and recently reported mixed-ligand amino complexes 75

  II (OH)/O 2 and Z-Cu II (NO 3 )) and two different Cu I complexes (Cu I (NH 3 ) 2 and Cu I (NH 3 )O fw ) were combined and labelled with Z-Cu(II) and Cu(I), while the mobile mixed ligand complex Cu II (NH 3 ) 3 X is labelled with m-Cu(II) (the temperature profiles for all five principle components are reported in Figure S11 of SI). One can see that at high temperature (400 o C and 450 o C) both monometallic Cu-CZC and bimetallic Cu-Fe-mixed samples dominated by the contributions from framework interacting Z-Cu(II) complexes, being slightly less abundant for Cu-CZC sample that is compensated by the higher concentration of framework interacting Z-Cu(I) complex. This result is in correlation with the lower magnitude of the 1 st shell maximum in FT-EXAFS amplitudes (reported in Figure 6b) -CZC sample with respect to the mixture. The lower reducibily of Cu sites in Cu-Fe-mix at high temperatures could be explained by the presence of small Fe 2 O 3 clusters (likely formed on exterior surface of Fe-MOR) that effeciently catalize NH 3 oxidation 37, 38 and thus prevent the formation of Z-Cu(I) complexes. At T = 100 o C almost the same ratio between Z-Cu(II) and m-Cu(II) species accompanied by small contribution (below 5%) from the mobile Cu(I) species is observed for Cu-CZC and Cu-Fe-mix samples. As discussed above, the most significant difference in Cu-speciation between Cu-CZC and Cu-Fe mixture has been observed at low-medium temperatures Indeed, in the range of 150 to 300 o C the Cu-Fe-mix catalysts is dominated by the contributions from mobile linear amino-complexes Cu(I) with the abundancy ca. 45 %. For Cu-Fe-mix catalyst the maximum contribution from mobile Cu(I) was obtained at 200 o C, with abundancy up to ca. 52 %, while for monometallic Cu-CZC at the same temperature only ca. 24%. For Cu-CZC component the maximum abundancy for Cu(I) component was obtained at 300 o C, that is contributed both by mobile di-amino and framework coordinated Cu(I) species (See Figure S12 of SI).

  o C) with respect to monometallic copper catalysts. Considering for the very low NO conversion obtained for pure iron catalyst (⁓ 4.5% at 150 o C and ⁓ 16.5% at 200 o C) the Fe-MOR counterpart can be roughly considered as spectator in Cu-Fe-mix catalyst at low temperature range.

Figure 7

 7 Figure 7 Relative abundance temperature profile for different Cuspecies formed in the monometallic Cu-CZC (a) and mechanical mixture Cu-Fe-mix (b) catalysts under NH3-SCR conditions, derived by XANES linear combination analysis. (c) Difference in relative abundancy of framework-coordinated Z-Cu II and Cu I sites in mechanical mixture and monometallic Cu-CZC samples.

12 |

 12 J. Name., 2012, 00, 1-3 This journal is © The Royal Society of Chemistry 20xx

  .e. pore size and availability) and Si/Al ratio. Maier et al. also showed an effect of Fe loading on the abundancy of Fe 2 O 3 oxides in a series of Fe-BEA catalysts via ex situ Mössbauer characterization

		39 . Based on the lack of Fe-Fe contribution
	and the presence of Fe-Al contribution resulting in a
	coordination number around 1, Choi et al., proposed the
	formation of monomeric Z-[Fe(O 2 )]	+ and Z-[Fe(OH) 2 ] as a
	dominant iron site under He or CO atmosphere. Such species
	are almost unaffected by the Fe:Al ratio.
	Forde et al.	35 demonstrated the Fe-Fe contribution to the
	EXAFS signal has been found for Fe-ZSM-5 and Cu-Fe-ZSM-5
	catalysts with Fe loading ca. 4% calcined at 550	o C in air. The
	authors proposed the formation of iron oligomers with a
	Fe 3+ /Fe 2+ in octahedral coordination or a small Fe 2 O 3 cluster.
	The critical iron loading to form an isolated iron species inside
	the zeolites was reported to be around 0.2 wt% of Fe	40 .
	However, this value may vary depending on framework
	topology (i

41

.

Table 1 .

 1 Summary of physochemical properties of the parent and metal exchanged zeolites.

	Catalyst label	(Al+P)/Si	Cu/Si	M content*(wt. %)	SBET (m 2 /g)	Vmic(cm 3 /g)
	Cu-CZC	11.24	0.44	1.56	568	0.19
	Catalyst label	Si/Al	Fe/Al	M content*(wt. %) a	SBET(m 2 /g)	Vmic(cm 3 /g)
	MOR parent	6.30	-	-	453	0.15
	Fe-MOR	6.60	1.43	7.55	483	0.17

22

.

  or due to the distortion of the O h sites upon heating. Likewise, non-ideal average octahedral coordination of the Fe species in the sample before activation could be a reason of higher pre-edge peak intensity observed at RT with respect to α-Fe(III) 2 O 3 , where Fe-sites are supposed to have almost perfect octahedral coordination O h 3+ .

Thereby it could be considered as an evidence of a small Fe-O clusters formation with highly defective structure of α-Fe 2 O 3 due to the size effect. The formation of the dominant fraction of Fe-O clusters with a local atomic structure similar to γ-Fe 2 O 3 (Maghemite) or Fe 3 O 4 (Magnetite) is excluded because of mismatch of the experimental XANES signal obtained for the activated sample with the spectra of γ-Fe 2 O 3 and Fe 3 O 4 reported elsewhere 53

  , we suggest that iron sites in both onecomponent Fe-MOR and two-component Cu-Fe-mix samples are represented by two main categories: small Fe 2 O 3 clusters most likely deposited on the exterior MOR surface and the minority of isolated Fe 3+ in T h coordination or highly distorted O h coordination. The later might be in the form of Fe

		3+
	monomers that replace framework Al and represent highly
	active sites for high temperature SCR in accordance with the
	literature	34, 57, 61 , while major fraction of Fe atoms form small
	Fe 2 O 3 clusters that efficiently catalyze NH 3 oxidation 37, 38

showed that a dual layer with a thinner Fe-ZSM-5 layer on top

Acknowledgements

The authors acknowledge ESRF (beamline BM23) for allocation of beamtime. The research was financially supported by the Ministry of Science and Higher Education of the Russian Federation (State assignment in the field of scientific activity, № 0852-2020-0019). The authors declare no conflict of interests.

***

Conflicts of interest

There are no conflicts to declare.